#------------------------------------------------------------------------------
#$Date: 2022-02-01 10:54:27 +0200 (Tue, 01 Feb 2022) $
#$Revision: 272380 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/56/62/1566227.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1566227
loop_
_publ_author_name
'Vladislav V. Gurzhiy'
'Alina R. Izatulina'
'Maria G. Krzhizhanovskaya'
'Mikhail N. Murashko'
'Dar-ya V. Spiridonova'
'Vladimir V. Shilovskikh'
'Sergey V. Krivovichev'
_publ_section_title
;
 Thermal behavior of uranyl selenite minerals derriksite and
 demesmaekerite
;
_journal_name_full               'Journal of GeoSciences'
_journal_page_first              249
_journal_page_last               259
_journal_paper_doi               10.3190/jgeosci.315
_journal_volume                  65
_journal_year                    2020
_chemical_formula_moiety         'Cu4 H6 O14 Se2 U'
_chemical_formula_sum            'Cu4 H6 O14 Se2 U'
_chemical_formula_weight         880.16
_space_group_crystal_system      orthorhombic
_space_group_IT_number           31
_space_group_name_Hall           'P 2ac -2'
_space_group_name_H-M_alt        'P m n 21'
_atom_sites_solution_hydrogens   difmap
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.9702(2)
_cell_length_b                   5.5629(3)
_cell_length_c                   19.0733(8)
_cell_measurement_reflns_used    2487
_cell_measurement_temperature    233(2)
_cell_measurement_theta_max      30.5550
_cell_measurement_theta_min      3.8040
_cell_volume                     633.46(5)
_computing_cell_refinement       'CrysAlisPro 1.171.39.44a (Rigaku OD, 2018)'
_computing_data_collection       'CrysAlisPro 1.171.39.44a (Rigaku OD, 2018)'
_computing_data_reduction        'CrysAlisPro 1.171.39.44a (Rigaku OD, 2018)'
_computing_molecular_graphics    'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2018/3 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXT 2018/3 (Sheldrick, 2015)'
_diffrn_ambient_environment      N~2~
_diffrn_ambient_temperature      233(2)
_diffrn_detector                 'CCD plate'
_diffrn_detector_area_resol_mean 10.3829
_diffrn_detector_type            Atlas
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_details
;
List of Runs (angles in degrees, time in seconds):

  # Type    Start    End  Width  tₑₓₚ   ω     θ     κ     φ   Frames
--------------------------------------------------------------------------
  1  ω    -47.00   3.00   1.00   22.50    --  -14.99  77.00-180.00   50
  2  ω    -27.00  19.00   1.00   22.50    --  -14.99 -77.00-150.00   46
  3  ω     42.00  83.00   1.00   22.50    --   16.86 178.00 -30.00   41
  4  ω     31.00  59.00   1.00   22.50    --   16.86 -99.00 120.00   28
  5  ω     -4.00  93.00   1.00   22.50    --   16.86  38.00 120.00   97
  6  ω     -8.00  93.00   1.00   22.50    --   16.86  38.00  30.00  101
;
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'SuperNova, Dual, Cu at home/near, Atlas'
_diffrn_measurement_method       'ω scans'
_diffrn_orient_matrix_type
'CrysAlisPro convention (1999,Acta A55,543-557)'
_diffrn_orient_matrix_UB_11      0.1097603000
_diffrn_orient_matrix_UB_12      0.0391996000
_diffrn_orient_matrix_UB_13      0.0084410000
_diffrn_orient_matrix_UB_21      -0.0303399000
_diffrn_orient_matrix_UB_22      0.1196510000
_diffrn_orient_matrix_UB_23      -0.0085824000
_diffrn_orient_matrix_UB_31      -0.0338260000
_diffrn_orient_matrix_UB_32      0.0197864000
_diffrn_orient_matrix_UB_33      0.0351315000
_diffrn_radiation_monochromator  mirror
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0431
_diffrn_reflns_av_unetI/netI     0.0401
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.999
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -7
_diffrn_reflns_limit_k_max       6
_diffrn_reflns_limit_k_min       -7
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_limit_l_min       -24
_diffrn_reflns_number            5136
_diffrn_reflns_point_group_measured_fraction_full 0.973
_diffrn_reflns_point_group_measured_fraction_max 0.970
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.472
_diffrn_reflns_theta_min         3.576
_diffrn_source                   'micro-focus sealed X-ray tube'
_diffrn_source_type              'SuperNova (Mo) X-ray Source'
_exptl_absorpt_coefficient_mu    25.163
_exptl_absorpt_correction_T_max  0.995
_exptl_absorpt_correction_T_min  0.990
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.39.44a (Rigaku Oxford Diffraction, 2018)
Analytical numeric absorption correction using a multifaceted crystal
			model based on expressions derived by R.C. Clark & J.S. Reid.
(Clark, R. C. & Reid, J. S. (1995). Acta Cryst. A51, 887-897)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            green
_exptl_crystal_density_diffrn    4.614
_exptl_crystal_description       prism
_exptl_crystal_F_000             788
_exptl_crystal_size_max          0.108
_exptl_crystal_size_mid          0.06
_exptl_crystal_size_min          0.041
_refine_diff_density_max         1.271
_refine_diff_density_min         -1.267
_refine_diff_density_rms         0.232
_refine_ls_abs_structure_details
;
 Flack x determined using 667 quotients [(I+)-(I-)]/[(I+)+(I-)]
 (Parsons, Flack and Wagner, Acta Cryst. B69 (2013) 249-259).
;
_refine_ls_abs_structure_Flack   -0.034(19)
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.043
_refine_ls_hydrogen_treatment    refxyz
_refine_ls_matrix_type           full
_refine_ls_number_parameters     117
_refine_ls_number_reflns         1546
_refine_ls_number_restraints     7
_refine_ls_restrained_S_all      1.041
_refine_ls_R_factor_all          0.0380
_refine_ls_R_factor_gt           0.0368
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0639P)²] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0902
_refine_ls_wR_factor_ref         0.0913
_reflns_Friedel_coverage         0.888
_reflns_Friedel_fraction_full    0.946
_reflns_Friedel_fraction_max     0.940
_reflns_number_gt                1493
_reflns_number_total             1546
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            Derriksite_SN_-40C_last.cif
_cod_data_source_block           derriksite_sn_-40C
_cod_database_code               1566227
_chemical_oxdiff_formula         'Cu4 U Se2 O14'
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_reflns_odcompleteness_completeness 99.70
_reflns_odcompleteness_iscentric 1
_reflns_odcompleteness_theta     28.51
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.5 times of:
  All O(H) groups
2. Restrained distances
 O9-H9
 1 with sigma of 0.02
 H9-O5_$5
 2.15 with sigma of 0.02
 O7-H7
 0.9 with sigma of 0.02
 O10-H10
 0.9 with sigma of 0.02
 O8-H8
 0.95 with sigma of 0.02
 H8-O1_$3
 2.1 with sigma of 0.02
3. Uiso/Uaniso restraints and constraints
Uanis(O7) = Uanis(O10)
4. Others
 Fixed Sof: H9(0.5)
;
_olex2_submission_special_instructions 'No special instructions were received'
_oxdiff_exptl_absorpt_empirical_details
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
;
_oxdiff_exptl_absorpt_empirical_full_max 3.326
_oxdiff_exptl_absorpt_empirical_full_min 0.557
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, -y, z+1/2'
'x+1/2, -y, z+1/2'
'-x, y, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
U1 U 0.500000 0.18523(15) 0.60652(5) 0.0158(2) Uani 1 2 d S T P . .
Se1 Se 0.000000 -0.1403(5) 0.52736(11) 0.0179(5) Uani 1 2 d S T P . .
Se2 Se 1.000000 0.5085(4) 0.68992(11) 0.0160(5) Uani 1 2 d S T P . .
Cu1 Cu -0.2501(2) 0.6055(3) 0.36174(10) 0.0090(4) Uani 1 1 d . . . . .
Cu2 Cu 0.000000 0.1101(4) 0.35382(15) 0.0080(5) Uani 1 2 d S T P . .
Cu3 Cu -0.500000 0.1011(4) 0.35615(15) 0.0077(4) Uani 1 2 d S T P . .
O1 O 0.500000 0.460(4) 0.5568(10) 0.033(4) Uani 1 2 d S T P . .
O2 O 0.500000 -0.084(4) 0.6556(9) 0.032(4) Uani 1 2 d S T P . .
O3 O 0.219(2) 0.060(3) 0.5345(6) 0.026(3) Uani 1 1 d . . . . .
O4 O 0.000000 -0.203(3) 0.4426(8) 0.012(3) Uani 1 2 d S T P . .
O5 O 0.780(2) 0.310(3) 0.6822(7) 0.028(3) Uani 1 1 d . . . . .
O6 O 1.000000 0.557(3) 0.7754(8) 0.013(3) Uani 1 2 d S T P . .
O7 O -0.2534(17) 0.276(2) 0.4022(5) 0.0084(13) Uani 1 1 d D . . . .
H7 H -0.24(3) 0.25(4) 0.448(3) 0.013 Uiso 1 1 d D U . . .
O8 O -0.500000 0.722(3) 0.4147(8) 0.009(3) Uani 1 2 d DS T P . .
H8 H -0.500000 0.62(3) 0.457(6) 0.014 Uiso 1 2 d DS U P . .
O9 O 0.000000 0.487(3) 0.3085(8) 0.010(3) Uani 1 2 d DS T P . .
H9 H 0.07(3) 0.55(6) 0.265(7) 0.015 Uiso 0.5 1 d D U P . .
O10 O -0.2484(13) -0.0720(19) 0.3125(6) 0.0084(13) Uani 1 1 d D . . . .
H10 H -0.24(3) -0.09(4) 0.266(2) 0.013 Uiso 1 1 d D U . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Se Se -0.0929 2.2259 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
U U -9.6767 9.6646 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_exptl_crystal_face_index_h
_exptl_crystal_face_index_k
_exptl_crystal_face_index_l
_exptl_crystal_face_perp_dist
-3 1 25 0.0213
-8 0 1 0.0487
8 0 5 0.0396
-2 5 19 0.0250
1 7 -11 0.0187
2 -4 -21 0.0323
-1 -7 10 0.0219
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 U1 O3 86.7(6) . .
O1 U1 O3 86.7(6) . 4_655
O1 U1 O5 94.2(6) . 4_655
O1 U1 O5 94.2(6) . .
O2 U1 O1 179.7(10) . .
O2 U1 O3 93.4(6) . 4_655
O2 U1 O3 93.4(6) . .
O2 U1 O5 85.6(6) . .
O2 U1 O5 85.6(6) . 4_655
O3 U1 O3 95.0(6) 4_655 .
O3 U1 O5 86.3(4) . 4_655
O3 U1 O5 178.5(5) 4_655 4_655
O3 U1 O5 178.5(5) . .
O3 U1 O5 86.3(4) 4_655 .
O5 U1 O5 92.4(7) 4_655 .
O3 Se1 O3 98.7(9) . 4
O4 Se1 O3 102.3(6) . .
O4 Se1 O3 102.3(6) . 4
O5 Se2 O5 99.6(10) . 4_755
O6 Se2 O5 100.9(6) . .
O6 Se2 O5 100.9(6) . 4_755
O4 Cu1 Cu1 51.5(2) 1_565 4
O4 Cu1 O6 175.4(5) 1_565 2_564
O6 Cu1 Cu1 128.4(2) 2_564 4
O7 Cu1 Cu1 90.6(3) . 4
O7 Cu1 O4 99.6(5) . 1_565
O7 Cu1 O6 85.0(5) . 2_564
O7 Cu1 O10 175.2(5) . 1_565
O8 Cu1 Cu1 141.2(4) . 4
O8 Cu1 O4 89.7(4) . 1_565
O8 Cu1 O6 90.3(4) . 2_564
O8 Cu1 O7 95.7(6) . .
O8 Cu1 O9 179.7(6) . .
O8 Cu1 O10 87.1(5) . 1_565
O9 Cu1 Cu1 39.0(4) . 4
O9 Cu1 O4 90.5(4) . 1_565
O9 Cu1 O6 89.5(5) . 2_564
O9 Cu1 O7 84.1(5) . .
O9 Cu1 O10 93.2(5) . 1_565
O10 Cu1 Cu1 89.7(2) 1_565 4
O10 Cu1 O4 84.3(5) 1_565 1_565
O10 Cu1 O6 91.1(5) 1_565 2_564
O7 Cu2 O4 90.5(4) . .
O7 Cu2 O4 90.5(4) 4 .
O7 Cu2 O7 98.4(6) 4 .
O7 Cu2 O9 75.4(4) . .
O7 Cu2 O9 75.4(4) 4 .
O9 Cu2 O4 158.2(5) . .
O10 Cu2 O4 84.8(4) . .
O10 Cu2 O4 84.8(4) 4 .
O10 Cu2 O7 81.5(4) 4 4
O10 Cu2 O7 81.5(4) . .
O10 Cu2 O7 175.4(5) . 4
O10 Cu2 O7 175.4(5) 4 .
O10 Cu2 O9 108.9(4) . .
O10 Cu2 O9 108.9(4) 4 .
O10 Cu2 O10 98.3(6) 4 .
Cu3 Cu3 Cu2 0(10) 4_455 1_455
Cu3 Cu3 O7 0(10) 4_455 4_455
Cu3 Cu3 O7 0(10) 4_455 .
Cu3 Cu3 O8 0(10) 4_455 1_545
Cu3 Cu3 O10 0(10) 4_455 .
Cu3 Cu3 O10 0(10) 4_455 4_455
O7 Cu3 Cu2 138.1(3) . 1_455
O7 Cu3 Cu2 41.6(3) 4_455 1_455
O7 Cu3 O7 96.6(6) . 4_455
O7 Cu3 O8 103.2(4) 4_455 1_545
O7 Cu3 O8 103.2(4) . 1_545
O8 Cu3 Cu2 91.24(7) 1_545 1_455
O10 Cu3 Cu2 139.9(3) . 1_455
O10 Cu3 Cu2 40.5(3) 4_455 1_455
O10 Cu3 O7 82.0(4) . .
O10 Cu3 O7 178.4(5) 4_455 .
O10 Cu3 O7 178.4(5) . 4_455
O10 Cu3 O7 82.0(4) 4_455 4_455
O10 Cu3 O8 76.4(4) . 1_545
O10 Cu3 O8 76.4(4) 4_455 1_545
O10 Cu3 O10 99.5(6) 4_455 .
Se1 O3 U1 143.6(8) . .
Se1 O4 Cu1 136.3(4) . 1_545
Se1 O4 Cu1 136.3(4) . 4_545
Se1 O4 Cu2 122.1(8) . .
Cu1 O4 Cu1 77.0(5) 1_545 4_545
Cu1 O4 Cu2 82.5(4) 4_545 .
Cu1 O4 Cu2 82.5(4) 1_545 .
Se2 O5 U1 142.8(8) . .
Se2 O6 Cu1 127.9(6) . 2_565
Se2 O6 Cu1 127.9(6) . 3_665
Cu1 O6 Cu1 76.9(5) 3_665 2_565
Cu1 O7 Cu2 103.9(5) . .
Cu1 O7 H7 121(10) . .
Cu2 O7 H7 107(10) . .
Cu3 O7 Cu1 106.8(5) . .
Cu3 O7 Cu1 106.8(5) 4_455 .
Cu3 O7 Cu2 97.5(5) . .
Cu3 O7 Cu2 97.5(5) 4_455 .
Cu3 O7 Cu3 0.00(19) 4_455 .
Cu3 O7 H7 117(10) . .
Cu3 O7 H7 117(10) 4_455 .
Cu1 O8 Cu1 102.4(7) 4_455 .
Cu1 O8 Cu3 93.0(5) 4_455 1_565
Cu1 O8 Cu3 93.0(5) . 1_565
Cu1 O8 H8 104(7) . .
Cu1 O8 H8 104(7) 4_455 .
Cu3 O8 H8 152(10) 1_565 .
Cu1 O9 Cu1 102.0(7) . 4
Cu1 O9 Cu2 96.7(5) . .
Cu1 O9 Cu2 96.7(5) 4 .
Cu1 O9 H9 130(10) . .
Cu1 O9 H9 90(10) 4 .
Cu2 O9 H9 130(10) . .
Cu1 O10 H10 112(10) 1_545 .
Cu2 O10 Cu1 106.0(5) . 1_545
Cu2 O10 Cu3 98.9(5) . 4_455
Cu2 O10 Cu3 98.9(5) . .
Cu2 O10 H10 115(10) . .
Cu3 O10 Cu1 103.5(4) 4_455 1_545
Cu3 O10 Cu1 103.5(4) . 1_545
Cu3 O10 Cu3 0.0(2) 4_455 .
Cu3 O10 H10 120(10) 4_455 .
Cu3 O10 H10 120(10) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
U1 O1 1.80(2) .
U1 O2 1.76(2) .
U1 O3 2.279(12) 4_655
U1 O3 2.279(12) .
U1 O5 2.314(13) 4_655
U1 O5 2.314(13) .
Se1 O3 1.720(13) .
Se1 O3 1.720(13) 4
Se1 O4 1.653(15) .
Se2 O5 1.722(13) .
Se2 O5 1.722(13) 4_755
Se2 O6 1.652(15) .
Cu1 Cu1 2.987(3) 4
Cu1 O4 2.398(12) 1_565
Cu1 O6 2.400(13) 2_564
Cu1 O7 1.988(11) .
Cu1 O8 1.914(9) .
Cu1 O9 1.922(10) .
Cu1 O10 2.025(11) 1_565
Cu2 O4 2.428(16) .
Cu2 O7 1.999(11) 4
Cu2 O7 1.999(11) .
Cu2 O9 2.268(15) .
Cu2 O10 1.961(10) .
Cu2 O10 1.961(10) 4
Cu3 Cu3 0.000(6) 4_455
Cu3 O7 1.972(11) 4_455
Cu3 O7 1.972(11) .
Cu3 O8 2.386(16) 1_545
Cu3 O10 1.969(9) 4_455
Cu3 O10 1.969(9) .
O7 H7 0.90(3) .
O8 H8 0.97(3) .
O9 H9 1.00(3) .
O10 H10 0.90(3) .
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
O3 Se1 O3 U1 109.1(12) 4 . . .
O3 Se1 O4 Cu1 64.8(12) . . . 4_545
O3 Se1 O4 Cu1 166.7(11) 4 . . 4_545
O3 Se1 O4 Cu1 -166.7(10) . . . 1_545
O3 Se1 O4 Cu1 -64.8(12) 4 . . 1_545
O3 Se1 O4 Cu2 50.9(5) 4 . . .
O3 Se1 O4 Cu2 -50.9(5) . . . .
O4 Se1 O3 U1 -146.2(12) . . . .
O5 Se2 O5 U1 -106.8(12) 4_755 . . .
O5 Se2 O6 Cu1 -0.9(10) . . . 2_565
O5 Se2 O6 Cu1 0.9(10) 4_755 . . 3_665
O5 Se2 O6 Cu1 -103.1(8) 4_755 . . 2_565
O5 Se2 O6 Cu1 103.1(8) . . . 3_665
O6 Se2 O5 U1 149.9(12) . . . .
loop_
_exptl_oxdiff_crystal_face_indexfrac_h
_exptl_oxdiff_crystal_face_indexfrac_k
_exptl_oxdiff_crystal_face_indexfrac_l
_exptl_oxdiff_crystal_face_x
_exptl_oxdiff_crystal_face_y
_exptl_oxdiff_crystal_face_z
-2.6320 1.2167 25.1936 -0.0104 -0.0042 0.9999
-8.4076 0.1667 0.5799 -0.9197 0.2163 0.3277
8.2525 0.1046 5.1923 0.9666 -0.2289 -0.1150
-2.1224 5.1811 18.9871 0.1177 0.5188 0.8467
0.8673 7.0849 -11.0871 0.2241 0.9358 -0.2721
2.3067 -4.3550 -21.0966 -0.0902 -0.4047 -0.9100
-0.7693 -7.2103 10.1697 -0.2262 -0.9456 0.2339
